received: 15 November 2015 accepted: 01 February 2016 Published: 18 February 2016
Tailoring nonlinear optical properties of Bi2Se3 through ion irradiation Yang Tan1, Zhinan Guo3,4, Zhen Shang1, Fang Liu2, Roman Böttger2, Shengqiang Zhou2, Jundong Shao3,4, Xuefeng Yu4, Han Zhang3 & Feng Chen1 The nonlinear optical property of topological insulator bismuth selenide (Bi2Se3) is found to be welltailored through ion irradiation by intentionally introducing defects. The increase of the optical modulation depth sensitively depends on the careful selection of the irradiation condition. By implementing the ion irradiated Bi2Se3 film as an optical saturable absorber device for the Q-switched wave-guide laser, an enhanced laser performance has been obtained including narrower pulse duration and higher peak power. Our work provides a new approach of tailoring the nonlinear optical properties of materials through ion irradiation, a well-developed chip-technology, which could find wider applicability to other layered two-dimensional materials beyond topological insulators, such as graphene, MoS2, black phosphours etc. Two-dimensional (2D) materials have received great scientific and technical attentions in research areas of physics, chemistry, and materials sciences1,2. In optics, peculiar optical performances have been found in 2D materials including polarization dependent absorption and nonlinear optical absorption3–5. Besides, 2D materials can be easily integrated with photonic structures such as waveguides and cavities, since the surfaces of 2D materials can be passivated without any dangling bonds. Based on the unique optical properties of 2D materials, many important optical applications have been realized in integrated photonics, including waveguide polarizers, mode-locked, waveguide amplifier6 and Q-switched waveguide lasers3,7–11. Taking the Q-switched pulsed waveguide laser for example, a waveguide structure with doping of rare-earth ions could be used as the gain medium and 2D materials with the saturable absorption property can be coated onto the waveguide facet as broadband optical saturable absorbers. Properties of 2D materials can be tailored by doping and external electric field. Recently, it has been demonstrated that the ion irradiation can also induce beneficial effects to nanostructured materials12–15. The interaction of energetic particles (e.g. electrons or ions) normally generates atomic defects in the target and changes properties of the materials. In spite of defects, the ion irradiation process may bring a positive effect to the material, in some cases. For example, the atomic constitution and morphology of graphene can be changed in a controllable manner by ion irradiation16. For nanotubes, ion irradiation can interconnect and merge the nanotubes, induce extreme pressure and lead to the formation of fullerene like “onions” in the nanotube17. In addition, it has been proved that the mechanical, electronic and even magnetic properties of nanostructured materials can be tailored by ion irradiation18–20. Nevertheless, there have been no reports on tailoring the optical properties of 2D materials by ion irradiation as of yet. The Bi2Se3 film, as a prototype topological insulator (TI), possesses an excellent saturable absorption and has been applied in Q-switched laser as the saturable absorber21,22. In this work, we applied the ion irradiation to modify the nonlinear optical property of the Bi2Se3 film in constructive way. The Bi2Se3 films have been irradiated 1
School of Physics, State Key Laboratory of Crystal Materials and Key Laboratory of Particle Physics and Particle Irradiation (Ministry of Education) Shandong University Shandong, Jinan, 250100, China. 2Helmholtz-Zentrum Dresden-Rossendorf, Institute of Ion Beam and Materials Research, Bautzner Landstrasse 400, 01328 Dresden, Germany. 3SZU-NUS Collaborative Innovation Center for Optoelectronic Science and Technology, Key Laboratory of Optoelectronic Devices and Systems of Ministry of Education and Guangdong Province, College of Optoelectronic Engineering, Shenzhen University, Shenzhen 518060, P.R. China. 4Institute of Biomedicine and Biotechnology, Shenzhen Institutes of Advanced Technology, Chinese Academy of Sciences, Shenzhen 518055, P.R. China. Correspondence and requests for materials should be addressed to Y.T. (email: [email protected]
) or H.Z. (email: [email protected]
) or F.C. (email: [email protected]
) Scientific Reports | 6:21799 | DOI: 10.1038/srep21799
Figure 1. Bi2Se3 nanoplatelets. SEM image (a) and the XRD diffraction pattern (b) of Bi2Se3 NPs. with nitrogen ions to diverse, precisely controlled fluences. It has been found that the saturable absorption of the Bi2Se3 film was enhanced after irradiation. The modification of the nonlinear optical absorption has shown a direct relation to the irradiation-induced defects in Bi2Se3. Through a careful control of the defect concentration, the saturable absorption of Bi2Se3 was intentionally tailored. The irradiated Bi2Se3 film was integrated with a neodymium doped yttrium aluminum garnet (Nd:YAG) waveguide for the passively Q-switched waveguide laser generation. Based on the modulation of the irradiated Bi2Se3 film, the Q-switched pulses with shorter pulse duration and a higher peak power were obtained, demonstrating the advantages of the irradiation treatment on the optical properties of 2D materials.
Results and Discussion
Bi2Se3 nanoplatelets. The Bi2Se3 nanoplatelets (NPs) used in the current study were synthesized via a polyol method. During the Bi2Se3 NPs synthesis, multiple reagents were added into a 25.0 mL two-neck flask with a teflon-coated magnetic stirring bar, including 0.10 g of bismuth (III) nitrate pentahydrate (Bi(NO3)3⋅ 5H2O), 0.05 g of sodium selenite (Na2SeO3), 0.22 g of polyvinyl pyrrolidone (PVP), and 10.0 mL of ethylene glycol (EG). The flask was connected to a reflux condenser and heated by a heating mantle. After heating the solution to 190 oC for 2 hours under constant stirring, the flask was removed from the heating mantle and the Bi2Se3 NPs were chemically grown in the solution, the SEM image is shown in Fig. 1a. The XRD pattern of the Bi2Se3 NP is displayed in Fig. 1b indicating the good crystallinity of the as-produced NPs. Then, the solution was cooled, centrifuged, washed (with isopropyl alcohol), and dropped onto a silica wafer. Dried at 60 °C, the solution was volatilized and Bi2Se3 NPs overlapped with each other constituting a 2D material film on the silica wafer. The thickness of the Bi2Se3 film was measured to be 180 nm (± 5 nm) by the atomic force microscope (AFM). Optical properties of irradiated Bi2Se3 films. Three pieces of Bi2Se3 films were irradiated by N+ ions at
a series of fluences, which were labeled as S1 (1 × 1012 ions/cm2), S2 (1 × 1013 ions/cm2) and S3 (1 × 1014 ions/cm2), respectively. One piece of the Bi2Se3 film without irradiation was used as the control/reference sample (S0). The measured nonlinear transmission of Bi2Se3 films is shown in Fig. 2. As we can see, the clear saturable absorption of the Bi2Se3 films was observed in all three samples. However, there are remarkable differences in the nonlinear transmission induced by ion irradiation in S1, S2 and S3. The modulation depth (Δ T) and the saturable intensity (Isat) of the Bi2Se3 films are increased with the irradiation fluence. To quantitatively determine the saturable absorption property of Bi2Se3 film, the relation between the transmission (T) and the excitation energy (I) has been fitted by the following formula23: − I I sat
T ( I ) = 1 − ∆T × e
where TN is the nonsaturable absorbance. The fitted values of the optical parameters are shown in Fig. 2e,f. Δ T and Isat of the original sample (S0) are 12.9% and 0.4 GW, respectively. The value of Isat can be tailored by the fluence of N+ ions. In the case of low-fluence irradiation (less than 1 × 1013 ions/cm2), Isat has a rapid change. By further increasing the ion fluence, the variation is smaller and tends to saturation. For the modulation depth, there is a sensitive response of the Bi2Se3 film to the irradiation treatment at the low-fluence regime. And the value of Δ T is adjusted from 12.9% to 19% by the fluence. With a fluence of more than 1 × 1013 ions/cm2, Δ T reaches a saturation value of 19%. Based on the previous discussion, the saturable absorption of the Bi2Se3 film can be tailored by ion irradiation. Utilizing the irradiated Bi2Se3 film as the saturable absorber, the performance of the Q-switched pulse laser is expected to be improved. For example, the pulse duration of the Q-switched pulse laser can be expressed by the equation below24,25: τp ≈
Scientific Reports | 6:21799 | DOI: 10.1038/srep21799
3.52T R ∆T
Figure 2. Optical properties of irradiated Bi2Se3 films. Nonlinear transmission as a function of the probe light intensity of S0 (a), S1 (b), S2 (c) and S3 (d). Color solid lines are fitted curves. Black lines in (a–c) are fitted curves of S0 for comparison. Color bands are error bands (± 2.5%). The modulation depth (e) and the saturable intensity (f) of the irradiated Bi2Se3 film under different fluence.
where τp is the pulse duration and TR is the cavity round-trip time. A shorter pulse duration can be obtained by increasing the modulation depth. Besides, the saturable intensity of the Bi2Se3 film is increased after irradiation. Therefore, a higher energy of the excitation laser is required in order to reach the saturation of the irradiated Bi2Se3 film, suggesting that the pulse energy of the Q-switched pulse laser can be further increased.
Mechanism of tailoring the nonlinear optical properties. In order to explain the mechanism of tailored nonlinear optical properties, the Raman spectra of Bi2Se3 films were measured by a confocal microscope. Figure 3a shows the measured Raman spectra and the variation of the E2g peak with respect to different irradiation fluences. As one can see, phonon peaks have blue shifts and their intensity is decreased. The change of the phonon peak (E2g) directly relates to the ion fluence. The variation of the Raman spectra indicates the deformation or damage of the Bi2Se3 structure by the ion irradiation. During the irradiation process, the incident energetic ions lost their energy, which was transferred from nitrogen ions to the host atoms in the Bi2Se3 film and caused the displacement of atoms in the Bi2Se3 (defects/damage Scientific Reports | 6:21799 | DOI: 10.1038/srep21799
Figure 3. Raman spectra of irradiated Bi2Se3 film. (a) Raman spectra of S0, S1, S2, and S3. The peak intensity (b) and peak position (c) variation of E2g with the fluence.
Figure 4. Mechanism of tailoring the nonlinear optical properties. (a) The relative atom displacement of the irradiated Bi2Se3 films along with the depth. (b,c) are the variation rate of the modulation depth (circles) and the saturable intensity (squares) with different relative atom displacement.
of the structure) through both inelastic and elastic collisions with the host atoms (also known as electronic and nuclear energy losses). The amount of structural damage in the Bi2Se3 film can be calculated by the Monte Carlo simulation SRIM (Stopping and Range of Ions in Matter)26. To simplify the discussion, the irradiation-induced structure damage is numerically represented by the relative atom displacement (RAD) in the Bi2Se3 film (percentage of the disordered atoms in the Bi2Se3 film). Figure 4a shows the distribution of RAD along with the depth from the sample surface towards to the bulk. The damage induced by irradiation is different along the depth and is concentrated near the surface (depth less than 80 nm). Besides, the damage is nearly proportional to the ion fluence of irradiation. Increasing the ion fluence from 1 × 1012 to 1 × 1014 ions/cm2, the average RAD of the Bi2Se3 is increased by two orders of magnitude, that is, 0.025% (S1), 0.247% (S2) and 2.467% (S3), respectively. The relationship between the average RAD of the Bi2Se3 and the nonlinear optical parameters is displayed in Fig. 4b,c. With the damage less than 0.25%, Δ T and Isat have a rapid change and the amplitudes of the variation are 1.4% and 3.2%, respectively. At high-damage level (more than 0.25%), the value of parameters tends to saturate. According to the relationship between the RAD and the nonlinear optical property (the saturable absorption), the optical performance of the Bi2Se3 can be precisely controlled by irradiation. The interaction between the incident ions and the Bi2Se3 film can be simulated by SRIM. And the calculated RAD can give us a rough conjecture of the nonlinear optical properties of the irradiated Bi2Se3.
Scientific Reports | 6:21799 | DOI: 10.1038/srep21799
Figure 5. Application of the irradiated Bi2Se3 film. (a) Nonlinear transmission of ST0 (red circles) and ST3 (blue circles). (b) Experimental setup for the Q-switched pulse waveguide laser. The variation of the pulse duration (d), modulation depth (e) and peak power (f) as a function of the pumping power, modulated by ST0 (red circles) and ST3 (blue circles), respectively.
Ion irradiation has been demonstrated as a novel method to tailor the nonlinear optical property of the Bi2Se3 film. Through the control of the ion fluence, the saturable absorption properties can be modulated efficiently. This work suggests that ion irradiation is an efficient way to modify the nonlinear optical property of 2D materials, which suggests broad applications in ultrafast laser photonics. Utilizing the ion-irradiated Bi2Se3 films as the optical saturable absorbers, the performance of the Q-switched waveguide laser is supposed to be enhanced. In this work, the irradiated Bi2Se3 film was utilized as the passive saturable absorber for the Q-switched waveguide laser emission. In order to reduce the saturable intensity of the film, S3 was thinned by the mechanical exfoliation. The material near the surface of S3 was removed and the remaining Bi2Se3 has a thickness of 10 nm (labeled as ST3). According to the simulation result shown in Fig. 4a, the average RAD in ST3 was 0.01%. S0 was also thinned to the 10 nm by the same technology as the control sample (labeled as ST0). The measured nonlinear transmissions of ST0 and ST3 are shown in Fig. 5a. The saturable intensity and the modulation depth of ST0 are found to be 4.7 MW/cm2 and 5%, respectively. In ST3, the values of Isat and T are increased by a factor of 1.76 and 1.22, respectively. The variation rates of optical parameters in ST3 are pointed in Fig. 4b,c (the red square and the pink triangle, respectively). As one can see, the measured values of ST3 show a good agreement with previous results. The experimental setup for the Q-switched waveguide laser is shown in Fig. 5b. ST1 and ST0 were compressed onto the output facet of a Nd:YAG waveguide as the saturable absorber, respectively. With the pumping power above 300 mW at 810 nm, a stable pulse laser emission is observed under the modulation of ST0 and ST3, respectively. The pulse trains of the output laser are shown in Fig. 5c under a pumping power of 350 mW. The pulse duration and the peak power of the output laser are shown in Fig. 5d,e, respectively. According to the measured pulse duration, the modulation depth can be calculated by Equation (2) and is displayed in Fig. 5e. The pulse laser modulated by ST3 has a higher peak power and larger modulation depth than ST0 under the same pumping condition. The measured parameters of the output pulse laser demonstrate the better performance of the irradiated Bi2Se3 as the saturable absorber, such as a higher peak power and a shorter pulse duration.
Ion irradiation. Four pieces of Bi2Se3 films were prepared by the same technology for this work. Three of them
were irradiated by N+ ions with an energy of 30 keV at different fluences, labeled as S1 (fluence of 1 × 1012 ions/cm2), S2 (fluence of 1 × 1013 ions/cm2) and S3 (fluence of 1 × 1014 ions/cm2), respectively.
Nonlinear transmission measurement. The nonlinear absorption coefficient of the Bi2Se3 film was measured by the Z-scan technology. A 1064-nm laser with 22-ps pulse duration and an energy of 0.5 μ J was focused using a lens (a focal distance of 400 mm), resulting in ∼ 24.5 μ m beam waist. For an accurate measurement, a large-aperture lens was used for collecting the transmitted laser light. By moving the Bi2Se3 film to the focal point, the power of the transmitted light was measured as a function of the energy density of the probe light. Mechanical exfoliation of the Bi2Se3 film. The Bi2Se3 was mechanically exfoliated by the ordinary adhesive tape: Lightly pasting the tape onto the surface of the Bi2Se3 film and then uncovering the adhesive tape. The Scientific Reports | 6:21799 | DOI: 10.1038/srep21799
www.nature.com/scientificreports/ Bi2Se3 will stick to the surface of the tape and be stripped. After repeating this operation, the thickness of the Bi2Se3 will be reduced to the desired thickness.
Q-switched waveguide laser. Figure 4b shows the schematic for the generation of Q-switched waveguide
lasers. The waveguide structure was fabricated by the femtosecond laser writing27. The double-cladding waveguide was inscribed into a neodymium doped yttrium aluminum garnet (Nd:YAG) ceramic sample (doped by 2% Nd3+ ions, offered by Baikowski Ltd.). The diameters of the inner and outer tubular cladding are 30 μ m and 100 μ m, respectively. The detailed information of the waveguide fabrication was reported in ref. 28. The Nd:YAG ceramic waveguide was used as the gain medium for the laser emission at the wavelength of 1064 nm. A mirror with a reflectivity of 99.98% was coated onto the input facet of the waveguide as the input mirror. While, a Bi2Se3 film was compressed tightly onto the output facet. The resonant cavity was composed by the Nd:YAG ceramic waveguide, the input mirror and the Bi2Se3 film. A continuous-wave optical pump at the wavelength of 810 nm was utilized in this work from a tunable Ti:Sapphire laser (Coherent MBR PE). The pump beam was focused by a convex lens (focal length 25 mm) and coupled into the Nd:YAG ceramic waveguide passing through the input mirror. As the Q-factor of this resonant cavity was modulated by the saturable absorption of the Bi2Se3 film on the output facet, the emission of the pulsed waveguide laser can be obtained.
1. Xia, F., Wang, H., Xiao, D., Dubey, M. & Ramasubramaniam, A. Two-dimensional material nanophotonics. Nat. Photon. 8, 899–907 (2014). 2. Fiori, G. et al. Electronics based on two-dimensional materials. Nat. Nanotechnol 9, 768–779 (2014). 3. Bao, Q. et al. Broadband graphene polarizer. Nat. Photon. 5, 411 (2011). 4. Fu, X., Qian, J., Qiao, X., Tan, P. & Peng, Z. Nonlinear saturable absorption of vertically stood WS2 nanoplates. Opt. Lett. 39 6450 (2014). 5. Wang, Y. et al. Ultrafast recovery time and broadband saturable absorption properties of black phosphorus suspension. Appl. Phys. Lett. 107, 091905 (2015). 6. Tan, Y. et al. Bi2Se3 Q-switched Nd:YAG ceramic waveguide laser. Opt. Lett. 40, 637 (2015). 7. Tan, Y. et al. Swift carbon ion irradiated Nd:YAG ceramic optical waveguide amplifier. Opt. Express 21, 13992–13997 (2013). 8. Tan, Y., Akhmadaliev, S., Zhou, S. Q., Sun, S. Q. & Chen, F., Guided continuous-wave and graphene-based Q-switched lasers in carbon ion irradiated Nd:YAG ceramic channel waveguide. Opt. Express 22, 3572–3577 (2014). 9. Choudhary, A. et al. 456-mW graphene Q-switched Yb:yttria waveguide laser by evanescent-field interaction. Opt. Lett. 40, 1912–1915 (2015). 10. Choi, S. Y. et al. Q-switched operation of a femtosecond-laser-inscribed Yb:YAG channel waveguide laser using carbon nanotubes. Opt. Express 23, 7999 (2015). 11. Kim, J. W. et al. Graphene Q-switched Yb:KYW planar waveguide laser. AIP Advances 5, 017110 (2015). 12. Peng, B. et al. Measurements of near-ultimate strength for multiwalled carbon nanotubes and irradiation-induced crosslinking improvements. Nat. Nanotechnol. 3, 626 (2008). 13. Smith, B. W., Monthioux, M. & Luzzi, D. E. Encapsulated C60 in carbon nanotubes. Nature 396, 323 (1998). 14. Kis, A. et al. Reinforcement of single-walled carbon nanotube bundles by intertube bridging. Nat. Mater. 3, 153 (2004). 15. Gómez-Navarro, C. et al. Tuning the conductance of single-walled carbon nanotubes by ion irradiation in the Anderson localization regime. Nat. Mater. 4, 534 (2005). 16. Cruz-Silva, E. et al. Controlling Edge Morphology in Graphene Layers Using Electron Irradiation: From Sharp Atomic Edges to Coalesced Layers Forming Loops. Phys. Rev. Lett. 105, 045501 (2010). 17. Sun, l. Krasheninnikov, A. V., Ahlgren, T., Nordlund, K. & Banhart, F. Plastic Deformation of Single Nanometer-Sized Crystals. Phys. Rev. Lett. 101, 156101 (2008). 18. Terrones, M. et al. Molecular junctions by joining single-walled carbon nanotubes. Phys. Rev. Lett. 89, 075505 (2002). 19. Sun, L. et al. P. M. Carbon nanotubes as high-pressure cylinders and nanoextruders. Science 312, 1199–1202 (2006). 20. Sun, l. Krasheninnikov, A. V., Ahlgren, T., Nordlund, K. & Banhart, F. Plastic Deformation of Single Nanometer-Sized Crystals. Phys. Rev. Lett. 101, 156101 (2008). 21. Zhao, C. et al. Ultra-short pulse generation by a topological insulator based saturable absorber. Appl. Phys. Lett. 101, 211106 (2012). 22. Wang, B. et al. Optimization of Q-switched Lasers. J. IEEE Photonics J. 6, 1501007 (2015). 23. Du, J. et al. Ytterbium-doped fiber laser passively mode locked by few-layer Molybdenum Disulfide (MoS2) saturable absorber functioned with evanescent field interaction. Sci. Rep. 4, 6346 (2014). 24. Zayhowski, J. J. & Kelley, P. L. Optimization of Q-switched Lasers IEEE J. Quantum Electron. 27, 2220–2225 (1991). 25. Spühler, G. J. et al. Experimentallyconfirmed design guidelines for passively Q-switched microchip lasers using semiconductor saturableabsorbers. J. Opt. Soc. Am. B 16, 376–388 (1999). 26. Ziegler, James, F. The stopping and range of ions in matter (2015). Available at www.srim.org (Accessed: 25th April 2015). 27. Chen, F. & Vazquez de Aldana, J. R. Optical waveguides in crystalline dielectric materials produced by femtosecond- laser micromachining. Laser Photonics Rev. 8, 251–275 (2014). 28. Tan, Y., Luan, Q., Liu, F., Chen, F. & Rodríguez Vázquez de Aldana, J. Q-switched pulse laser generation from double-cladding Nd:YAG ceramics waveguides Opt. Express 21, 18963–18968 (2013).
This research work is supported by the following funding programs: National Natural Science Foundation of China (Grant No. 11535008, by F. C. and Grant Nos 61435010, 61435010 and 61222505 by H. Z.), Young Scholars Program of Shandong University (Grant No. 2015WLJH20 by Y. T.) and Helmholtz Association (VH-NG-713 by S. Z.). Ion irradiation has been performed at the Ion Beam Center at the Helmholtz-Zentrum Dresden – Rossendorf.
Y.T., H.Z. and F.C. conceived the idea and designed the work. Z.G., J.S., X.Y. and H.Z. fabricated Bi2Se3 films. F.L., R.B. and S.Z. performance the ion irradiation. Y.T., Z.S. and F.C. performed rest experiments and simulations. All the authors discussed the results and participated in the manuscript preparation.
Competing financial interests: The authors declare no competing financial interests. Scientific Reports | 6:21799 | DOI: 10.1038/srep21799
www.nature.com/scientificreports/ How to cite this article: Tan, Y. et al. Tailoring nonlinear optical properties of Bi2Se3 through ion irradiation. Sci. Rep. 6, 21799; doi: 10.1038/srep21799 (2016). This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
Scientific Reports | 6:21799 | DOI: 10.1038/srep21799